## Surface and interstitial Ti diﬀusion at the rutile TiO

### 2

## (110) surface

## w

### P. A. Mulheran,*

a### M. Nolan,*

b### C. S. Browne,

c### M. Basham,

d### E. Sanville

e### and

### R. A. Bennett

fReceived 8th February 2010, Accepted 20th May 2010

DOI: 10.1039/c002698k

Diﬀusion of Ti through the TiO2(110) rutile surface plays a key role in the growth and

reactivity of TiO2. To understand the fundamental aspects of this important process, we

present an analysis of the diﬀusion of Ti ad-species at the stoichiometric TiO2(110) surface

using complementary computational methodologies of density functional theory corrected for on-site Coulomb interactions (DFT +U) and a charge equilibration (QEq) atomistic potential to identify minimum energy pathways. We ﬁnd that diﬀusion of Ti from the surface to subsurface (andvice versa) follows an interstitialcy exchange mechanism, involving exchange of surface Ti with the 6-fold coordinated Ti below the bridging oxygen rows. Diﬀusion in the subsurface between layers also follows an interstitialcy mechanism. The diﬀusion of Ti is discussed in light of continued attempts to understand the re-oxidation of non-stoichiometric TiO2(110)

surfaces.

### 1.

### Introduction

Titanium dioxide is a technologically important material and
has garnered considerable attention as a possible source of
clean energy by photocatalytic water splitting, as a cleanup
technology in waste streams and when combined with suitable
supported metal catalysts as an environmental gas puriﬁer.
Titania also has applications in coatings and sensors.1_{Besides}

these applications, it is one of the most widely studied proto-typical reducible metal oxides with the Ti having many stable oxidation states producing a complex structural phase diagram.2 Stoichiometric TiO2 has four polymorphs: rutile, anatase,

brookite and cotunnite.3 _{Nearly stoichiometric rutile shows}

two homologous series of planar bulk defects that self-assemble into crystallographic shear planes: TinO2n1with (4ono10)

based on {121} directed planes, and (16onoB37) based on {132}.4–6 Stable reduced phases down to Ti4O7, a crystal

structure with promising electrical characteristics,7 _{can}

also be formed. Ti2O3 is a corundum structured pure Ti3+

phase which also appears as a reduced surface phase on near

stoichiometric rutile surfaces treated in vacuum.8_{The }

equili-brium phases make an interesting system in which to modify the electrical and structural characteristics of the oxide. The atomistic processes that allow the system to move, for example, from stoichiometric rutile to a self-assembled planar array of defects in the bulk upon reduction, are somewhat hidden from view. However, recent experimental work has highlighted some key constituents to the puzzle, notably by considering the reverse process, that is the re-oxidation of non-stoichiometric material.9–11

The rutile (110) surface has been extensively investigated
experimentally over a number of years by surface science
techniques, and usually on electrically conducting bulk reduced
crystals that have changed colour which indicates a
non-stoichiometry. Early work on re-oxidation by Henderson
suggested Ti interstitials were the key point defect in
non-stoichiometric rutile.12_{Indeed Scanning Tunnelling Microscopy}

(STM) studies by Onishi and Iwasawa showed how these defects can move from bulk to surface to grow new surface phases, the so-called added row Ti2O3 reconstruction.8 At

elevated temperature, however, variable temperature STM revealed how the (110) surface of a reduced crystal re-grows new layers of TiO2(in contrast to Ti2O3) in a rather complex

layer-by-layer fashion when exposed to oxygen.9,10 These
studies show that the reduced crystal contains a solid solution
of Ti interstitials that are mobile above B473 K and able
to diﬀuse to the surface to react with the impinging oxygen
(or other adsorbed species such as formate13_{). The relationship}

between the reduction and re-oxidation steps has been
demon-strated by further experiments on the self-doping of titania
crystals and ultra-thin ﬁlms which show how deposited Ti
adatoms can diﬀuse into the bulk as interstitials when annealed.14
Ti interstitials and adatoms are therefore of paramount
impor-tance to the surface structures,15_{the surface chemistry}16_{and}

the growth of titania, and it is desirable to have modelling schemes that can describe these species, their reactivity and their mobility.17 Modelling schemes that accurately represent

a

Department of Chemical and Process Engineering, University of Strathclyde, 75 Montrose Street,

Glasgow G1 1XJ, UK. E-mail: paul.mulheran@strath.ac.uk; Fax: +44 (0)141 548 2539; Tel: +44 (0)141 548 2385

b_{Tyndall National Institute, University College Cork, Lee Maltings,}

Cork, Ireland. E-mail: michael.nolan@tyndall.ie; Fax: +353 21-4270271; Tel: +353 21-490-4063

c

Department of Physics, University of Reading, Whiteknights, Reading, RG6 6AF, UK

d

Diamond Light Source Ltd, Diamond House, Harwell Science and Innovation Campus, Didcot OX11 0DE, UK

e

Department of Mathematical Sciences, Loughborough University, Loughborough LE11 3TU, UK

f_{School of Chemistry, University of Reading, Whiteknights,}

Reading RG6 6AD, UK. E-mail: r.a.bennett@reading.ac.uk; Fax: +44 (0)1189750203; Tel: +44 (0)1183788559

w_{Electronic supplementary information (ESI) available: Bader charge}

analysis of Ti adatom and interstitial structures, discussion of QEq potential and its modiﬁcation and experimental XPS data. See DOI: 10.1039/c002698k

electronic and geometric structures are particularly challenging for non-stoichiometric materials with variable oxidation states.

The description of reduced rutile has been an active topic for many years, with much discussion as to whether the dominant species involved are Ti interstitials15 or oxygen vacancies.18 Both defects can produce the same signature in ultraviolet photoemission spectroscopy and in density functional theory (DFT) simulations,19 i.e. reduced Ti3+ ions. However, this debate is not the reason we study Ti interstitials. Rather, given that these species are key to the growth of TiO2through their

diﬀusion from bulk to the surface and reaction with oxygen, we are studying the diﬀusion of Ti interstitials as a ﬁrst step to providing a deeper understanding of this process.

Ref. 17 provides a thorough exploration of the diﬀusion of Ti and O ad-species on the rutile (110) surface using density functional theory (DFT) with the local density approximation (LDA). However, it is known that this approach will not describe well the localisation of d-electrons that are expected in reduced titania. Therefore we have undertaken a series of calculations using DFT +Uto correct for on-site Coulomb interactions, providing a good comparator for the LDA results and allowing confrontation with experiment to assess the relative merits of the approaches.

In particular, in recent work we have presented direct
experimental validation of the DFT + U computational
approach, applied in this paper. We studied self-doped titania
ﬁlms, characterising the electronic properties of surface
adsorbed Ti.20We found that an approach such as DFT +U
is indeed needed to interpret the experimental results and
consistently describe the Ti3+ ions present in this system.
The best agreement with the spectroscopy of the gap states
induced by the adsorbed adatom is obtained withU= 3 eV.
This result is consistent with the value of U assigned in
calculations of oxygen vacancies in the (110) surface,21_{which}

create a reduced surface Ti defect state in the band gap. These latter calculations share important similarities with B3LYP results22which also localise the Ti 3d states.

In this paper we employ experimentally benchmarked
calcu-lations of static structures20_{to consider the dynamical aspects}

of Ti adatom and interstitial mobility in the rutile (110) surface. We ﬁnd key barriers and transition pathways in the surface and subsurface regions and explore their electronic structure. The results are contrasted with those of ref. 17, and are found to be in much better agreement with experimental results. Furthermore, we believe the charge localisation we predict facilitates new physical insight into surface growth and reactivity.

In our work, the DFT +Umethodology is used to investi-gate the stability and properties of the Ti interstitials, since it is known to provide a consistent description of reduced Ti.20,21

To investigate the diﬀusion pathways between the various adatom and interstitial sites, of which there are many possibilities, we ﬁrst employ atomistic calculations using the charge equilibra-tion (QEq) methodology.17,23–31In order to provide a realistic set of minimum energy pathways (MEP) for full investigation with DFT + U, we consider the eﬀectiveness of the QEq approach in describing the energy landscape of the defects, and ﬁnd that some modiﬁcation to the original model is required. The modiﬁcation employed involves altering the

degree of charge transfer between species in the model, in particular restricting the transfer to Ti species only. This change is grounded in our analysis of the DFT +Ucalculations, and is consistent with experimental observations. With the modiﬁed potential shown to describe interstitial Ti consis-tently, we then screen a number of diﬀusion pathways, and select the most energetically favourable for further quantiﬁ-cation using constrained minimisation in DFT +U calcula-tions. The QEq approach has the appealing quality of being able to describe defects such as Ti interstitials and their diﬀusion and is an appropriate method to use for modelling of the dynamics of Ti diﬀusion and reaction with oxygen to ultimately study the dynamics of TiO2growth.

The layout of the paper is as follows. In the following section, we describe the computational methodologies. In Section 3 we present results, ﬁrst for the structures and energies of the interstitials and adatoms using the DFT +U and atomistic QEq calculations, and describe the impact of our charge transfer modiﬁcation on the latter. In Section 3.2 we present results for our Minimum Energy Pathways for diﬀusion in the selvedge. Discussions of our results, focussing on charge transfer during diﬀusion, follow in Section 4 along with conclusions for the implications of our results for experi-mental interpretation and future dynamical simulation of surface growth.

### 2.

### Methodology

2.1 DFT +Ucalculations

All our ﬁrst principles calculations are carried out in the framework of periodic plane wave density functional theory (DFT).32 In this approach, the valence electronic states are expanded in a basis of periodic plane waves, with an energy cut-oﬀ of 396 eV, while the core–valence interaction is treated using PAW potentials.33 The PW91 exchange–correlation functional is used throughout. The surface is modelled as a ﬁnite thickness slab model with three-dimensional periodicity. Surface slabs along the z-direction (perpendicular to the surface) are separated using a vacuum thickness ofB10 A˚. For the interstitial calculations, a single Ti is placed in two diﬀerent sites in the ﬁrst, second and third (bulk-like) sub-surface O–Ti–O layers. Full relaxation is performed, except for the bottom O–Ti–O unit. We refer to our previous work for details of the Ti adatoms adsorbed at the rutile (110) surface.20

The slab model is 6 O–Ti–O units deep with a (24) surface
cell expansion, minimising periodic defect–defect interactions,
and providing a concentration of adsorbed Ti atoms that
matches the coverage used in self-doping experiments.20
k-Point sampling is at theG-point and the Methfessel–Paxton
smearing scheme with a smearing parameter of 0.1 eV is used.
As discussed in the Introduction, an important aspect of
these calculations concerns the theoretical description of the
reduced Ti ions. Reduced Ti ions have partially occupied 3d
shells, which can be diﬃcult to describe with approximate
DFT exchange–correlation functionals.21,34–37_{It has already}

been demonstrated that the DFT +U approach38,39can be successfully applied to study non-stoichiometric TiO220,21,34–37

due to Dudarevet al.39_{as implemented in VASP is employed.}

The quantity (U J) is used, where J is the exchange parameter. However, since the system is not magnetic, we set Jto be zero, so that (UJ)U. From our previous work,20 Uis set to 3 eV.

The charge density from the converged VASP calculations was partitioned to the ions using our own Bader analysis code,40allowing comparisons to be made to the charge distri-butions predicted through the QEq approach described next.

2.2 QEq calculations

The DFT +Umethodology leads to stronger localisation of charges in non-stoichiometric or defective structures in com-parison to standard DFT.20,21This physical picture strengthens the possibility of using empirical potential schemes which employ charges ﬁxed spatially to ion cores in the lattice and especially those models which have the ﬂexibility to allow charges to move. One such leading scheme is the QEq methodology23which allows charge transfer between ions to minimise the electrostatic energyEes, whilst including

contri-butions from the charging energies for each ion which takes a parabolic form:

Ees=Si(E0i +w0iqi+Ji0q2i) +Si,jaiJijqiqj (1)

Here w0i andJ

0

i are related to the ions’ electronegativity and hardness.Jijis the shielded Coulomb interaction between ions, the shielding being estimated by the overlap of s-type Slater orbitals. For any given ionic conﬁguration, the charge qion the ions is adjusted to minimise eqn (1) under the constraint of conserved total charge Siqi = 0, without moving the ionic positions. Once this equilibration has been achieved, the resultant forces on the ions can be used to move them as in usual minimisation or dynamics procedures.25The atomistic model for the material is completed by the addition of short-range potentials to represent the covalent bonding which is known to be signiﬁcant for titania.1 Hallil et al. have developed a suitable model for titania, using a pair-functional form to describe Ti–O covalent bonds.28

In our QEq calculations we use the same rutile surface slabs described above for the DFT + U calculations. The lattice parameters were ﬁxed to bulk values, and the ion coordinates relaxed. For both DFT +Uand the QEq calculations, results with larger cells, larger vacuum gaps, and with two adsorbed adatoms either side of the slab (for the Ti adatom calculations) produce essentially identical results; more details are in ref. 20. The geometry minimisations were performed using a conjugate gradient method and we use our own in-house code to perform all the QEq calculations.

Minimum Energy Pathways for the interstitial and adatom diﬀusion are created with the QEq atomistic potential using the nudged elastic band method.41 Selected pathways are further investigated using constrained minimisation with DFT + U. Here the position of the migrating species is held ﬁxed whilst the surrounding atoms are relaxed. This procedure is performed for each image along the pathway, thereby assessing the pathway’s viability and obtaining another estimate of the activation energy.

### 3.

### Results

3.1 The structure and energy of interstitials in the (110) surface

In ref. 20 we presented results for the Ti adatom at the rutile (110) surface. Two stable binding sites are possible, the more favourable of which positions the adatom between two bridging and one in-plane oxygen. Due to the symmetry, we referred to it as theihsite.20In this paper, we ﬁnd it convenient to change our notation where this adsorption site will henceforth be labelled A; see Fig. 1. An alternative stable adsorption site is possible where the adatom is positioned between 2 in-plane and one bridging oxygen, labelled site B in Fig. 1 and throughout the paper (it was labelledivin ref. 20).

Within our DFT +Umethodology, we calculated that site A is 0.34 eV lower in energy than site B; however, a barrier for diﬀusion between B to A is present since B is found to be stable upon relaxation.

An important aspect of the DFT +Uapproach is to relate
the localisation of charge to the defect-induced gap state
observed in experiment. A convenient representation is found
by plotting the spin iso-surfaces for the four extra unpaired
d-electrons present in the surface with adsorbed Ti. Following
this scheme, we present in Fig. 2 the spin iso-surfaces with
interstitials in the ﬁrst, second and third O–Ti–O layers
beneath the (110) surface. These sites all have the same
symmetry as the adatom in site A. In Fig. 1 these sites are
indicated as Fi in the ﬁrst layer, and as shown they tend to sit
beneath in-plane oxygen in plan view rather than directly
beneath the site A adatom. The adatoms in the corresponding
site in layers 2 and 3 are referred to as Fii and Fiii in the
following section. The spin density plots in Fig. 2 show
reduced Ti ions present—in particular the interstitial Ti has
a Ti3+_{oxidation state and a small number of neighbouring Ti}

atoms are also reduced to Ti3+. Note that the electrons introduced by Ti are predominantly localised. In previous work, using hybrid DFT,42 Finazzi et al. also showed the formation of localised Ti3+ ions when a Ti interstitial is present, giving good conﬁdence in our use of DFT +U.

Fig. 1 Views of the (110) rutile surface indicating the adatom and interstitial sites used in this paper. Ti atoms are grey and O atoms are red. The bridging oxygen rows are indicated with the dashed lines. Site

A (and equivalents A0_{and D) is the adatom in its most favourable site,}

next to two bridging oxygen and one in-plane oxygen. Site B (and its equivalent E) is the adatom in its second favourable binding site next

to one bridging and 2 in-plane oxygen. Site Fiis an interstitial sitei

Also shown in Fig. 2 is the projected electron density of
states for the Fi interstitial site. This shows the defect-induced
gap state associated with Ti3+_{, arising from the interstitial}

atoms and reduction of neighbouring lattice Ti. This contrasts to the split level found for the adatom in site A, where a Ti2+signature is observed for the adatom, and a Ti3+feature for an in-plane ﬁve-fold coordinated Ti3+. In both cases, the remaining electron is spread across other lattice Ti. The corresponding results for the interstitial in the Bi site are not shown here but are broadly similar. They show surface 5-fold Ti reduced to 3+, the interstitial maintaining a 3+ oxidation state and the remaining charge spread over a small number of subsurface Ti.

We have also calculated the relaxed structure and energies of the interstitials using the QEq methodology.31In Fig. 3 we show the relative energetics for the Ti adatom and interstitials from DFT +Uand QEq calculations. With the energy of the A site adatom set to 0 eV for DFT +Uand QEq, the ﬁgure shows the relative energetics of the B site adatom and the

corresponding interstitial sites. Both DFT +Uand QEq ﬁnd the same stable sites, and furthermore the binding to the site A is the most favourable adatom site in both schemes, with an energy diﬀerence between A and B sites of 0.56 eV in the QEq scheme, respectively (cf.0.34 eV in DFT +U).

The diﬀerence in binding energy between the interstitial Fi and Bi sites (0.09 eV and 0.07 eV, respectively) is much less marked than that between A and B in both the DFT +Uand the QEq calculations, as might be anticipated since in bulk these sites would be identical by symmetry.

However, there is a marked diﬀerence between the energy of
the adatom (A, B) and interstitial (Fi, Bi) sites calculated
by DFT + U and the Hallil QEq model. The DFT + U
calculation shows the interstitials are more energetically
favourable than adatoms by 0.6 eV and 0.8 eV, respectively,
for the A and B sites, whereas the QEq diﬀerences are very
much larger at 2.5 eV and 3.0 eV. This is a signiﬁcant
diﬀerence in the energy landscapes of the models. Whilst our
ﬁnding that Ti interstitials are more energetically favourable
than adatoms agrees with experimental results for adatoms
diﬀusing down into the bulk upon annealing,14trapping them
in the bulk by such a large amount as 2.5 eV does not accord
with the re-growth of reduced rutile at elevated temperature,
even if oxygen ad-species promote the growth.9,10,15 _{We}

conclude that the empirical QEq potential of Hallil et al.28 overestimates the adsorption energy of the interstitials with respect to the adatom energy.

The reason for the discrepancy in the adatom–interstitial binding energy diﬀerences can be traced to the charge transfer occurring in the QEq potential at the (110) surface. In Fig. 4 we show the QEq charges on the ions in the relaxed structures with the adatom in the surface A and B sites and the ﬁrst layer interstitial Fi and Bi sites, as well as the labelling for Tables 1 and 2. In this ﬁgure, the radius of the ions reﬂects their excess charge (in e) over bulk values in order to provide a pictorial view of the charge distribution. For comparison, Bader analysis is used to partition the charge to the ions in the DFT + U results. The charges on the ions are given in

Fig. 2 The spin density plots from the DFT +Uinterstitials: (a) Fi, (b) Fii and (c) Fiii. Also shown in (d) is the projected electronic density of states, showing the Ti 3d derived gap state induced by the Fi interstitial.

Tables 1 and 2, and for clarity we also provide the pictorial view of the charge distributions for all calculations in the ESI.w Referring to Tables 1 and 2, it is clear that there is a qualitative diﬀerence between the behaviour of the Ti and the O atoms in the two approaches. In the case of the Ti, the QEq charges are broadly correlated with the Bader charges. In contrast, the distribution of charges on the O atoms do not correlate well between the calculations. In particular, the Bader analysis of the DFT + U reveals only small excess charges on the O atoms, within the limits of about 0.1e, whereas the QEq model gives a much wider range of excess O charges in the range of about0.4e.

This charging of the oxygen nearest-neighbours by the Ti interstitial in the QEq model causes a favourable decrease in electrostatic energy with small penalties in self-energy (see eqn (1)) and from the short range potential. These combine to lead to an elastic distortion in the surrounding lattice with ions moving closer together, screening the interstitials and signiﬁcantly lowering the total energy. The response of the Ti adatom does not show such a strong eﬀect since the adatom has fewer oxygen neighbours to charge.

The behaviour of the oxygen within the Hallil model suggests that the energetics of the QEq component underplay the costs of moving the charge both to and from the oxygen. To understand the consequences of this, we have repeated our calculations keeping the charge on all of the oxygens ﬁxed to their bulk value of 1.26e, with only the Ti ions able to transfer charge between themselves using the original charging self-energies.28We show in Fig. 3 how the energy landscape of the defects, measured relative to the energy of the adatom in site A in each model, is now in much better agreement with the DFT +Uresults.

In support of the physical basis of this modiﬁcation to the QEq model, experimental data for the core-level shifts in X-ray photoelectron spectroscopy of stoichiometric TiO2(110), Ti adatom doped TiO2(110), and added row

Ti2O3reconstructed TiO2(110) are presented in the ESI.wAll

cases show very similar O1s lineshapes with no spectral features attributable to large variances in oxygen charge state. This conﬁrms that the charge transfer to and from the oxygen

Fig. 4 (a) Hallil model QEq results for the A adatom site; (b) Hallil model QEq results for the B site; (c) Hallil model QEq results for the Fi site and (d) Hallil model QEq results for the Bi site. The oxygens are red and the titanium dark grey. The size of the ions in all images represents how

much excess charge dQ(e) is associated with the ion in comparison to its bulk charge (speciﬁcally radius scales as 1 + 1.3dQ). The values of dQ

for the labelled ions are given in Tables 1 and 2. Only a section of the full cell used in the calculations is shown for clarity, with the upper surface being the free one with the exposed bridging oxygen.

Table 1 The excess charge dQ, measured in units of e_{, over bulk}

values for the ions labelled in Fig. 4a and b using the Hallil QEq

potential, DFT +Uand ﬁxed O-charge QEq

Hallil QEq DFT +U Fixed O QEq

A adatom

T1 0.775 0.585 0.825

T2 0.215 0.074 0.348

T3 0.010 0.007 0.056

O1 0.370 0.127 0.0

O2 0.047 0.000 0.0

B adatom

T1 0.812 0.990 0.825

T2 0.109 0.399 0.130

T3 0.273 0.006 0.420

O1 0.343 0.139 0.0

O2 0.011 0.016 0.0

O3 0.355 0.073 0.0

Table 2 The excess charge dQ, measured in units of e, over bulk values for ions labelled in Fig. 4c and d due to interstitial insertion

Hallil QEq model DFT +U Fixed oxygen-charge QEq

Fi interstitial

T1 0.417 0.178 0.767

T2 0.166 0.072 0.025

T3 0.191 0.331 0.336

T4 0.091 0.047 0.286

T5 0.050 0.034 0.178

O1 0.288 0.065 0.0

O2 0.309 0.097 0.0

O3 0.279 0.087 0.0

O4 0.311 0.132 0.0

O5 0.415 0.091 0.0

Bi interstitial

T1 0.409 0.216 0.748

T2 0.269 0.445 0.438

T3 0.104 0.032 0.032

T4 0.032 0.014 0.189

T5 0.118 0.224 0.296

O1 0.284 0.105 0.0

O2 0.348 0.082 0.0

O3 0.337 0.079 0.0

O4 0.259 0.103 0.0

atoms of the TiO2(110) surface upon Ti adsorption predicted

by our calculations should be minimal.

3.2 Minimum energy pathways for Ti interstitial diﬀusion

Detailed results for NEB calculations of Ti diﬀusion with the QEq potentials have previously been presented in ref. 31, to which we refer for further details. A summary of the activation energies of feasible diﬀusion pathways is given in Table 3, obtained with the modiﬁed (ﬁxed oxygen charge) QEq model. From these, we select the most favourable pathways for further investigation with DFT +U.

The ﬁrst pathway we consider for the diﬀusion between adatom and ﬁrst layer interstitial is A–Fiviaexchange with a 6-fold coordinated lattice Ti underneath the bridging oxygen row. In Fig. 5 we show the energies of the images along the relaxed NEB pathway, using the starting site A adatom QEq energy as a convenient zero of energy. For alternate images

along the path, we apply the constrained minimisation in DFT +Uand plot the relaxed energies of the images along-side the original QEq values, using the DFT +Uenergy of site A as a convenient zero of energy. This procedure allows a direct comparison of a Minimum Energy Pathway in both models. It is apparent that the activation energy for the pathway is similar in both models (0.97 eV for the QEqversus 0.83 eV in DFT +U). Furthermore, the shape of the pathway energy plots is similar, indicating the QEq saddle point is geometrically similar to the DFT +Uone. For convenience, we also show in Fig. 5 the DFT +Ugeometry at some key points on the path and will return to this point in a later section.

Table 3 shows that an alternative low-energy pathway exists for adatoms to diﬀuse to interstitial sites, that of B–Bi via exchange with an in-plane 5-fold coordinated Ti in the surface trench. In Fig. 6 we again compare the MEP found using the NEB method and the modiﬁed QEq with that obtained using constrained minimisation in DFT +Ualong the same path-way, using the starting site B energies in each model as convenient zeros of energy. Again we note the similarity in the shapes of the energy plots along this pathway, lending conﬁdence that the empirical potential provides a pathway that is also feasible in the DFT + U methodology. The activation energy is lower in the QEq scheme at 0.47 eV compared to 0.66 eV for DFT + U. However, the energy landscape shows that the relative energy of site B over site A is higher in the modiﬁed QEq (0.98 eV) than in the DFT +U (0.31 eV). This high energy starting point has the eﬀect of distorting the pathway, lowering the activation energy and moving the saddle point towards the interstitial site Bi.

While diﬀusion from a surface B site has a lower activation barrier than from the A site, we need to follow migration of

Table 3 Energy barriers (eV) for the forward and backward moves found using the NEB method using the ﬁxed oxygen-charge variant of

the QEq model; the ﬁgures in brackets are for the DFT +Uestimates

(see text)

Forward Backward

A–Fi (exchange) 0.97 (0.83) 1.41 (1.40)

A–Fi (direct) 2.20 (—) 2.64 (—)

B–Bi (exchange) 0.47 (0.66) 1.94 (1.55)

B–Bi (direct) 0.96 (—) 2.43 (—)

Bi–Bii (exchange) 1.31 (1.00) 1.35 (0.60)

Bi–Bii (direct) 2.02 (—) 2.06 (—)

Fi–Fii (exchange) 1.31 (0.76) 1.53 (0.84)

A–B 1.12 (0.83) 0.14 (0.52)

A–D 3.49 (—) 3.49 (—)

B–E 1.83 (—) 1.83 (—)

Bi–Fi 0.81 (0.72) 0.77 (0.63)

the Ti adatom from the surface A site to the surface B site. To this end, Fig. 7 shows the MEP for an adatom diﬀusing between sites A and B, which has a barrier of 1.12 eV (QEq)/0.83 eV (DFT + U). This emphasises the point that site B has a rather high energy in the modiﬁed QEq model, compared to the DFT +Ucalculations (see above) and the computed energy barriers also indicate that diﬀusion from the A to the B site will not be a frequent event. Of particular

interest is whether this distorts the activation energy of the adatom to interstitial diﬀusion. In the modiﬁed QEq, the composite pathway A–B–Bi is dominated by the ﬁrst step with the activation energy 1.12 eV, a little higher than the activation energy of 0.97 eV for the aforementioned A–Fi interstitial move. In the DFT + U model, the composite pathway again is dominated by the A–B activation energy 0.83 eV, which is the same activation energy as for the A–Fi

Fig. 6 Minimum Energy Pathways for B–Bivia5-fold exchange. The structure indicated at selected steps along the MEP includes the DFT +U spin density to show how the charge localisation changes during the migration process.

Fig. 7 Intra-layer Minimum Energy Pathways from the surface A to surface B site. The structure indicated at selected steps along the MEP

interstitial move. Therefore it seems both pathways are competitive in our calculations, although the A–B–Bi pathway has two steps, whereas the A–Fi pathway has a single step. The preference appears to be for the A–Fi pathway, although A–B–Bi would be possible on experimental timescales at the relevant growth temperature4400 K.9,10

To complete our analysis of the interstitial diﬀusion at the surface, we also study the MEP in the models with subsurface diﬀusion (data not shown). The intra-layer Bi–Fi move in the ﬁrst subsurface layer corresponds to the B–A adatom move at the surface. Again the trends in the curves are satisfactorily correlated, showing an almost symmetric shape, with an activation energy of 0.72 eV from DFT + U, lower than in the surface A–B move. Table 3 shows a summary of the MEP’s including diﬀusion pathways between subsurface layers. The interstitial move Bi–Biiviaexchange with a lattice Ti is found to be favoured over the direct move. The DFT +Uactivation energy for this diﬀusion is 1.00 eV, comparing with 1.31 eV for the modiﬁed QEq. The Fi–Fii exchange diﬀusion pathway has a barrier of 0.76 eV in DFT +Uin good agreement with the value used in ref. 15. The pathways for out-diﬀusion of interstitials towards the surface from bulk are also given in the backwards pathway column of Table 3.

### 4.

### Discussion and conclusions

The results in this paper present a thorough picture of the interaction of Ti atoms with the rutile (110) surface and provide useful insights into the near surface diﬀusion of interstitial Ti. The Ti adatom is most stable in the surface A site. Although interstitial sites are determined to be more stable, there is a barrier for diﬀusion from the surface to the interstitial sites (andvice versa). The most favourable pathway is the surface A site to interstitial Fi site (andvice versa). In this pathway, the Ti adatom moves towards a 6-fold coordinated lattice Ti site, which in a concerted motion, moves to the interstitial site. For this pathway, Fig. 5 shows the structures of some intermediate steps, clearly showing the concerted motion of both the adatom and the lattice Ti.

In the insets of Fig. 5 we show the computed spin density for
critical steps. In the A site, the Ti adatom is in the +2
oxidation state, a surface 5-fold coordinated Ti atom is in
the +3 oxidation state and the remaining electron of the four
introduced by neutral Ti is spread over a small number of
Ti atoms. In the interstitial Fi site, the interstitial Ti and
surrounding reduced Ti atoms have a +3 oxidation state. At
the highest point on the MEP, we see that the originally 6-fold
coordinated Ti atom has moved towards the interstitial site
and has picked up some charge so that the original adatom
now has a +3 oxidation state as does a subsurface Ti atom
(the previously reduced 5-fold surface Ti atom is now a Ti4+
ion). A second, local, maxima in the MEP arises when the
adatom and two surface 5-fold coordinated Ti atoms have a
+3 oxidation state and the interstitial is a Ti4+ion. By the
ﬁnal stages, one of the surface Ti3+_{ions is oxidised to Ti}4+

and the interstitial Ti is now a Ti3+_{ion and the system relaxes}

to a lower energy conﬁguration.

Thus, the Ti diﬀusion pathway shows a number of changes of Ti oxidation states for the diﬀusing atoms and for

neighbouring Ti atoms. Our results show that the barrier in
the MEP arises at the point at which two (large) Ti3+_{ions are}

rather close to each other, which is an energetically unfavourable situation. Once past this step on the MEP, the reduced Ti atoms are no longer so close to each other and migration of Ti proceeds. It is interesting to note that the interstitials donate charge to the 5-fold Ti in the surface and that these electrons will be available to adsorbates to aid dissociative adsorption.13 For the re-oxidation of the surface by O2one may expect these

sites to be especially reactive and lead to the creation of O adatom adsorption close to the Ti interstitials. These may then facilitate the out-diﬀusion of Ti interstitials through the exchange pathways identiﬁed here modiﬁed by the more stable transition and ﬁnal states.

For the Ti diﬀusion pathways in Fig. 6 and 7, we also show the structure and spin densities at important points along the MEP. In all these migration pathways, we observe that the maximum in the barrier is obtained when reduced Ti species come closest to each other along the migration pathway.

We can compare the diﬀusion barriers we ﬁnd with DFT +Uto those found using bare DFT (LDA) in ref. 17. In that work, the barrier for the A–Fi interstitialcy move is 1.60 eV (compared to 0.83 eV here) and for the B–Bi inter-stitialcy move it is 1.76 eV (cf.0.66 eV). The contrast for the reverse moves, i.e. the out-diﬀusion of interstitials to the surface, is even more marked, since the interstitials are highly favoured energetically over adatoms in LDA by 1.91 eV (cf. 0.53 eV here). These contrasts appear to be due to the role electron localisation plays in stabilising the structures and diﬀusion pathways, and as stated above, the correct descrip-tion of this will be important to the understanding of surface dissociative adsorption. There is no doubt that experiments support the lower diﬀusion barriers found in the DFT +U calculations here. Indeed, some of these diﬀusion pathways have been (indirectly) measured. In particular a barrier of 0.440.06 eV was found for the in-diﬀusion of submonolayer of Ti deposited on near stoichiometric TiO2(110).11 This

measurement follows Ti3+core-level shifted features in photo-emission spectroscopy and is thus sensitive to diﬀusion through several monolayers (the escape depth of photoemitted electrons) but is in reasonable agreement with the lower energy pathways described here. The bulk diﬀusion has been previously calculated to follow an interstitialcy mechanism with a barrier of 0.225 eV (signiﬁcantly lower than the barrier of 0.37 eV along thec-axis).43

A comparison of results for the DFT + U and QEq descriptions of adsorbed Ti and Ti interstitials shows that the modiﬁed QEq potential gives results that are in reasonable agreement with the DFT +Uresults. The relative stabilities of the various adatom and interstitial sites are in good agreement, as are the charge distributions, as evidenced by plotting the Bader charges for the Ti adatom and interstitial sites. We aim to use the QEq model for studying the interaction of Ti with oxygen and the growth of TiO2layers, full simulation of which

substoichiometric Ti is present. In addition, the QEq potential can also be used for screening of potential structures and diﬀusion pathways for full simulation with ﬁrst principles approaches.

### Acknowledgements

PAM, CSB and MB acknowledge support from EPSRC grants EP/C524349 and GR/T18738 and the University of Reading, UK. MN acknowledges support from Science Foun-dation Ireland, ‘‘EMOIN’’ grant number SFI 09/SIRG/I1620 and computing resources provided by the SFI and Higher Education Authority Funded Irish Centre for High End Computing.

### Notes and references

1 U. Diebold,Surf. Sci. Rep., 2003,48, 53.

2 G. V. Samsonov, The Oxide Handbook, IFI/Plenum Press,

New York, 1982.

3 L. S. Dubrovinsky, N. A. Dubrovinskaia, V. Swamy, J. Muscat,

N. M. Harrison, R. Ahuja, B. Holm and B. Johansson,Nature,

2001,410, 653.

4 R. A. Bennett, S. Poulston, P. Stone and M. Bowker,Phys. Rev. B:

Condens. Matter Mater. Phys., 1999,59, 10341.

5 G. S. Rohrer, V. E. Henrich and D. A. Bonnell,Science, 1990,250,

1239.

6 G. S. Rohrer, V. E. Henrich and D. A. Bonnell,Surf. Sci., 1992,

278, 146.

7 M. Marezio, A. Gauzzi, F. Licci and E. Gilioli,Phys. C, 2000,338,

1.

8 H. Onishi and Y. Iwasawa,Phys. Rev. Lett., 1996,76, 791.

9 P. Stone, R. A. Bennett and M. Bowker,New J. Phys., 1999,1, 8.

10 R. D. Smith, R. A. Bennett and M. Bowker, Phys. Rev. B:

Condens. Matter Mater. Phys., 2002,66, 035409.

11 M. Bowker and R. A. Bennett,J. Phys.: Condens. Matter, 2009,21,

474224; M. Bowker and R. A. Bennett,J. Phys.: Condens. Matter,

2010,22, 059801.

12 M. A. Henderson,Surf. Sci., 1999,419, 174.

13 R. A. Bennett, P. Stone and M. Bowker,Faraday Discuss., 1999,

114, 267.

14 R. A. Bennett and N. D. McCavish,Top. Catal., 2005,36, 11.

15 S. Wendt, P. T. Sprunger, E. Lira, G. K. H. Madsen, Z. Li, J. Ø. Hansen, J. Matthiesen, A. Blekinge-Rasmussen, E. Lægsgaard,

B. Hammer and F. Besenbacher,Science, 2008,320, 1755.

16 R. A. Bennett, P. Stone and M. Bowker,Faraday Discuss., 1999,

114, 267.

17 E. J. Sanville, L. J. Vernon, S. D. Kenny, R. Smith,

Y. Moghaddam, C. Browne and P. Mulheran, Phys. Rev. B:

Condens. Matter Mater. Phys., 2009,80, 235308.

18 C. M. Yim, C. L. Pang and G. Thornton,Phys. Rev. Lett., 2010,

104, 036806.

19 C. Di Valentin, G. Paachioni and A. Selloni,J. Phys. Chem. C,

2009,113, 20543.

20 M. Nolan, S. D. Elliott, J. S. Mulley, R. A. Bennett, M. Basham

and P. A. Mulheran,Phys. Rev. B: Condens. Matter Mater. Phys.,

2008,77, 235424.

21 B. J. Morgan and G. W. Watson,Surf. Sci., 2007,601, 5034.

22 C. Di Valentin, G. Pacchioni and A. Selloni,Phys. Rev. Lett., 2006,

97, 166803.

23 A. K. Rappe and W. A. Goddard, J. Phys. Chem., 1991,95,

3358.

24 X. W. Zhou, H. N. G. Wadley, J.-S. Filhol and M. N. Neurock, Phys. Rev. B: Condens. Matter Mater. Phys., 2004,69, 035402.

25 V. Swamy and J. D. Gale,Phys. Rev. B: Condens. Matter Mater.

Phys., 2000,62, 5406.

26 V. Swamy, J. Muscat, J. D. Gale and N. M. Harrison,Surf. Sci.,

2002,504, 115.

27 B. S. Thomas, N. A. Marks and B. D. Begg, Phys. Rev. B:

Condens. Matter Mater. Phys., 2004,69, 144122.

28 A. Hallil, R. Te´tot, F. Berthier, I. Braems and J. Creuze,Phys. Rev.

B: Condens. Matter Mater. Phys., 2006,73, 165406.

29 B. S. Thomas and N. A. Marks,Phys. Rev. B: Condens. Matter

Mater. Phys., 2007,76, 167401.

30 A. Hallil, R. Te´tot, F. Berthier, I. Braems and J. Creuze,Phys. Rev.

B: Condens. Matter Mater. Phys., 2007,76, 167402.

31 P. A. Mulheran, C. S. Browne and Y. Moghaddam,Mol. Simul.,

2009,35, 532.

32 G. Kresse and J. Hafner,Phys. Rev. B: Condens. Matter, 1994,49,

14251; G. Kresse and J. Furthmu¨ller,Comput. Mater. Sci., 1996,6,

15.

33 P. E. Blo¨chl, Phys. Rev. B: Condens. Matter, 1994, 50, 17953;

G. Kresse and D. Joubert,Phys. Rev. B: Condens. Matter Mater.

Phys., 1999,59, 1758.

34 Y. F. Zhang, W. Lin, Y. Li, K. N. Ding and J. Q. Li,J. Phys.

Chem. B, 2005,109, 19270.

35 A. I. Poteryaev, A. I. Lichtenstein and G. Kotliar,Phys. Rev. Lett.,

2004,93, 086401.

36 R. Pentcheva and W. E. Pickett,Phys. Rev. B: Condens. Matter

Mater. Phys., 2006,74, 035112.

37 D. D. Cuong, B. Lee, K. M. Choi, H. S. Ahn, S. Han and J. Lee, Phys. Rev. Lett., 2007,98, 115503.

38 V. I. Anisimov, J. Zaanen and O. K. Andersen, Phys. Rev. B:

Condens. Matter, 1991,44, 943.

39 S. L. Dudarev, G. A. Botton, S. Y. Savrasov, C. J. Humphreys and

A. P. Sutton,Phys. Rev. B: Condens. Matter Mater. Phys., 1998,

57, 1505.

40 E. Sanville, S. D. Kenny, R. Smith and G. Henkelman,J. Comput.

Chem., 2007,28, 899.

41 G. Henkelman and H. Johnsson,J. Chem. Phys., 2000,113, 9978.

42 E. Finazzi, C. Di Valentin and G. Pacchioni,J. Phys. Chem. C,

2009,113, 3382.

43 H. Iddir, S. O¨g˘u¨t, P. Zapol and N. D. Browning,Phys. Rev. B: